
Structure  Method  Capacity  References 

Graphene coated by S particles  Heat mixing  400 mA h/g after 40 cycles  [24] 
Sandwichtype  Solutionmixing  505 mA h/g after 100 cycles  [25] 
S particles wrapped by graphene  Selfassembly  600 mA h/g after 100 cycles  [26] 
S particles in graphene  Oil/water system  620 mA h/g after 60 cycles at 1C  [27] 
—  Deposition from  950 mA h/g after 55 cycles  [28] 
Wrinkled laminar structure  Deposition from Na_{2}S_{2}O_{3}  667 mA h/g after 200 cycles  [29] 
S particles in graphene sheets  Deposition from Na_{2}S_{2}O_{3}  830 mA h/g after 50 cycles  [30] 
S in the pores of actived graphene  Meltdiffusion  1000 mA h/g after 60 cycles at 0.2C  [31] 
S particles on graphene  Melting diffusion  957 mA h/g after 50 cycles  [32] 
Ternary composites  In situ polymerization  560 mA h/g after 100 cycles  [33] 
Sandwichtype  Heat mixing  800 mA h/g after 100 cycles  [34] 
S in the porous graphene  Meltdiffusion  755 mA h/g at 0.1C  [35] 
